Comparison of polymerization shrinkage of pattern resins Sarah B. Gibbs, DDS, MDS,a Antheunis Versluis, PhD,b Daranee Tantbirojn, DDS, MS, PhD,c and Swati Ahuja, BDS, MDSd College of Dentistry, University of Tennessee Health Science Center, Memphis, Tenn Statement of problem. The dimensional stability, in particular polymerization shrinkage, of pattern resins affects the accuracy of implant prosthesis fabrication. Recently introduced photopolymerizing pattern resins are easy to use, but their shrinkage needs to be determined and compared with traditional autopolymerizing pattern resins. Purpose. The purpose of the study was to compare the polymerization shrinkage of photopolymerizing pattern resins with autopolymerizing pattern resins. Material and methods. Two autopolymerizing (DuraLay, GC Pattern resin) and 2 photopolymerizing (Primopattern LC Gel, Primopattern LC Paste) pattern resins were tested. The sample size was 10 for each group. Polymerization shrinkage was determined by measuring the change in area dimensions with image analysis. The percentage of volumetric shrinkage was calculated, and the results were statistically analyzed with ANOVA, followed by the Student-Newman-Keuls post hoc test (a¼.05). Results. The volumetric shrinkage values (%; mean standard deviation) for GC Pattern Resin were 5.72 0.89; for DuraLay, 5.07 1.36; for Primopattern LC Gel, 5.42 1.83; and for Primopattern LC Paste, 7.43 0.62. The volumetric shrinkage of the Primopattern LC Paste was signiﬁcantly higher than that of the other 3 materials. Conclusions. The photopolymerizing pattern resin in gel form (Primopattern LC Gel) had a similar shrinkage value to the autopolymerizing pattern resins (DuraLay and GC Pattern Resin). However, the photopolymerizing pattern resin in paste form (Primopattern LC Paste) shrank signiﬁcantly more than the other 3 materials tested. (J Prosthet Dent 2014;-:---)
Clinical Implications Clinicians should be aware that the photopolymerizing pattern resin in paste form has a higher shrinkage value than that of the traditional autopolymerizing pattern resins and the photopolymerizing pattern resin in gel form. The higher shrinkage may affect the accuracy of implant prosthesis fabrication.
The accurate transfer of implant position to working casts with the ultimate goal of passively ﬁtting implant prostheses is an important aspect of prosthodontics.1-3 A passively ﬁtting implant restoration can be achieved
by fabricating a cast with veriﬁed implant positions captured by means of impressions incorporating splinted copings or impression devices fabricated from autopolymerizing acrylic resins.4-6
The autopolymerizing acrylic resins commonly used for implant device fabrication are GC Pattern Resin (GC America) and DuraLay (Reliance Dental Mfg Co). Both these methacrylatebased pattern resins are supplied as
This study is based on a graduate thesis (June 2013). a
Former Resident, Department of Prosthodontics. Professor, Department of Bioscience Research, University of Tennessee Health Science Center. c Associate Professor, Department of Restorative Dentistry, University of Tennessee Health Science Center. d Adjunct Assistant Professor, Department of Prosthodontics, University of Tennessee Health Science Center. b
Gibbs et al
Volume powder and liquid that need mixing to initiate the polymerization reaction. In 2009, new pattern resins were introduced (Primopattern; Primotec), which have been described as “a light cured universal modeling resin, ready to use one-component-material, available as modeling gel and modeling paste.”7 In general, photopolymerizing materials have an advantage over their autopolymerizing counterparts because of their ease of handling and reduced fabrication time.8,9 All resin-based materials exhibit polymerization shrinkage. The polymerization shrinkage of pattern resins contributes to distortion in implant prosthesis fabrication9,10; this is a concern, because the production of high-quality restorations demands accuracy. Several methods have been used to determine the dimensional accuracy or polymerization shrinkage of acrylic resins.8,11-13 Cho and Chee8 measured dimensional accuracy as changes in gap distance between copings indexed with DuraLay, GC Pattern Resin, and a new photopolymerizing resin. With a combination of a dilatometer and an inductive transducer, Mojon et al11 found a 24-hour volumetric shrinkage of 7.9% for DuraLay resin. Danesh et al12 used a hydrostatic method to evaluate the volumetric shrinkage of lightpolymerizing and autopolymerizing resins for occlusal splints and reported
values ranging from 4.5% to 6.4%. A more recent study using a strain gauge technique found that GC Pattern Resin produced less microstrain than DuraLay II for splinting implant impressions.13 For their pattern resin, GC reports polymerization shrinkage of 0.36% after 30 minutes and 0.37% after 24 hours but does not specify the method used to determine the shrinkage.14 The shrinkage values reported by GC are relatively low compared with values reported for other resins.11,12 Shrinkage values can be affected by the method of measurement.15 For example, some resin-based materials exhibited a 0.33% ‘postgel’ shrinkage measured with a strain gauge technique while exhibiting a 1.76% ‘total’ shrinkage measured with a linometer.16 Postgel shrinkage is the portion of shrinkage responsible for shrinkage stresses, and total shrinkage is the overall change in dimension. For pattern resins, the total shrinkage is most relevant, because the overall dimensional changes of a device are more important than potential residual stresses in the polymerized resin. To date, no information regarding polymerization shrinkage of the photopolymerizing Primopattern resins has been published. In addition, the values of autopolymerizing pattern resins reported by different authors were not measured by using the same method and are not
necessarily comparable. The purpose of this study was to determine and compare the polymerization shrinkage of various pattern resins. In dental research, total shrinkage has been determined by measuring ﬂuid displacement (dilatometer),11,17 changes in density (buoyancy method),12,18 dimensional changes (measured with a 1-dimensional transducer),19 or optical techniques (analysis of before-and-after images).20 In this study, a new, simpler optical method that did not require any dedicated shrinkage measurement equipment was used to measure the change of a surface area projection. The null hypothesis was that the volumetric shrinkage values of photopolymerizing pattern resins do not differ from those of autopolymerizing pattern resins.
MATERIAL AND METHODS The total polymerization shrinkage of 4 pattern resins was determined. The materials were 2 autopolymerizing acrylic resins, DuraLay (Reliance Dental Mfg Co) and GC Pattern Resin (GC America); a photopolymerizing gel (Primopattern LC Gel; Primotec); and a photopolymerizing paste (Primopattern LC Paste; Primotec). The sample size was 10 per group. Manufacturers and material information are listed in Table I.
GC Pattern Resin
Primopattern LC Gel
Primopattern LC Paste
Reliance Dental Mfg Co
Powder: Methacrylate polymer Dialkyl phthalate Benzoyl peroxide Liquid: Methyl methacrylate
Powder: Polymethyl methacrylate Polyethyl methacrylate Dibenzoyl peroxide Liquid: Methyl methacrylate 2-Hydroxyethyl-Methacrylate
Acrylic resins Fillers Initiators
Neopentylglykol propoxylat-Diacrylat 7,7,9-(bzw 7,9,9) Trimethyl-4, 13-dioxo-3,14-dioxa-5, 12-diaza-hexadecan-1, 16-dioldimethacrylat
Hand molded paste
Paint brush method
Paint brush method
No mixing required
No mixing required
Liquid lot 012601 Powder lot 040706
Liquid batch 1205021 Powder batch 1006242
Information on DuraLay, Primopattern LC Gel, and Primopattern LC Paste is from material safety data sheets of respective products.
The Journal of Prosthetic Dentistry
Gibbs et al
1 A, DuraLay specimen on silicone platform (green). B, Shrinkage measurement setup, consisting of stereomicroscope with digital camera and imaging software. Monitor shows image capture screen and measurement display. For the autopolymerizing resins, a powder-to-liquid ratio of 0.5 g to 0.3 mL was used. This ratio was determined in a preliminary trial to give a clinically manageable consistency. The manufacturers of DuraLay and GC Pattern Resin describe a brush technique for creating resin patterns, in which a monomersoaked brush is used to pick up the polymer, but they do not provide recommended powder-to-liquid ratios.21 In this study, the premeasured powder was added to the premeasured liquid and hand spatulated for 45 seconds for DuraLay and 20 seconds for GC Pattern Resin. The mixing times were based on an assessment of workable consistency. The mixture was placed on a square silicone platform fabricated from a heavy body impression material (Aquasil; Dentsply
Caulk) set against a glass slide to achieve a very smooth surface (Fig. 1A). The pattern resin specimens formed a dome shape because of their consistency. The specimen dimensions were approximately 6 mm in diameter and a maximum of 2.5 mm in height in the center. The specimens were placed under a stereomicroscope (SZX16; Olympus) with digital camera (UC30; Olympus) (see Fig. 1B), and the prepolymerization images of the specimens were captured from above at 1 minute 30 seconds from the start of mixing (Fig. 2B). For the autopolymerizing resins, the postpolymerization images were made 20 minutes after the start of mixing (see Fig. 2B). The 20-minute measurement point represented when these pattern resins were ready to be used clinically.
Primopattern LC Gel was dispensed directly from its syringe onto the silicone platforms, and Primopattern LC Paste was dispensed with a plastic scoop. After the prepolymerization images were captured, the specimens were irradiated for 5 minutes with a small polymerization unit (Metalight Mini; Primotec) according to the manufacturer’s recommendations.22 The postpolymerization images were captured immediately after the 5 minutes of irradiation. By using imaging software (Stream Basic; Olympus Soft Imaging Solutions GmbH), a minimum of 80 points was traced around the perimeter of the prepolymerization and postpolymerization images to calculate each specimen’s circumferential area (see Fig. 2). The projected area shrinkage (A) was calculated by dividing the change in
2 A, Primopattern LC Gel specimen with area measurement at ﬁrst image captured (prepolymerization image). B, Same specimen with area measurement at second image captured (postpolymerization image).
Gibbs et al
Volume area ðA0 A1 Þ by the original area ðA0 Þ:
Pattern Resin, and Primopattern LC Gel were not signiﬁcantly different. ANOVA results are shown in Table III.
A ¼ ðA0 A1 Þ=A0
DISCUSSION Area shrinkage (A) was converted to percentage volumetric shrinkage (V%) by using the following formula (Table II):
The importance of using a pattern resin with the least amount of shrinkage for implant impression procedures lies in the need to accurately reproduce the implant position for deﬁnitive restorations.6,9 The ultimate goal is achieving an implant framework that exhibits a passive ﬁt without undue ﬁtting stresses that could be detrimental to connecting screws, abutments, or patient tissues.13 Clinicians are familiar with fabricating resin patterns with autopolymerizing resin and the brush technique and with the shrinkage behavior of such resins. The more recently introduced photopolymerizing resins offer handling characteristics that can be more convenient and reduce chair time.8,10 In gel form, the pattern resin is distributed in a syringe, whereas the paste form can accommodate larger amounts and can be molded by hand. The objective of this study was to investigate how the dimensional stability of these new photopolymerized pattern resins compared with the stability of the conventional autopolymerizing materials.
V% ¼ 1 ð1 AÞ3=2 100 The differences in shrinkage among the pattern resins were analyzed with 1-way ANOVA, followed by the Student-Newman-Keuls post hoc test (a¼.05).
RESULTS The volume percentage of total polymerization shrinkage (mean standard deviation) for GC Pattern Resin was 5.72 0.89, DuraLay 5.07 1.36, Primopattern LC Gel 5.42 1.83, and Primopattern LC Paste 7.43 0.62 (Fig. 3). One-way ANOVA indicated that there were signiﬁcant differences among the 3 groups (df¼3, F¼6.121, P¼.002). The volumetric shrinkage of the Primopattern LC Paste was signiﬁcantly higher than the other 3 materials (Student-Newman-Keuls). The shrinkage values for DuraLay, GC
All specimens exhibited shrinkage after setting. The volumetric shrinkage values of DuraLay, GC Pattern Resin, and Primopattern LC Gel were in the same range (5.07% to 5.72%), whereas Primopattern LC Paste had the highest shrinkage (7.43%). Therefore, the null hypothesis that no difference would be found between autopolymerizing and photopolymerizing pattern resins was partially accepted. The photopolymerizing pattern resin in gel form had the same shrinkage value as the autopolymerizing pattern resins, but the photopolymerizing pattern resin in paste form had signiﬁcantly higher shrinkage value. Both Primopattern products were polymerized for 5 minutes with the Metalight polymerization unit recommended by the manufacturer for best dimensional stability given their innovative cooling system. This study found that both Primopattern resins shrank and that the shrinkage values were equivalent or higher than those of the traditional autopolymerizing resins DuraLay and GC Pattern Resin. DuraLay and GC Pattern Resin are composed of polymethyl methacrylate (acrylic resin). According to the material safety data sheets, Primopattern LC Gel is composed of acrylic resin, ﬁllers, and initiator, similar to DuraLay and GC Pattern Resin. The formulation of
Shrinkage value conversions Volumetric shrinkage: DV=V0 ¼ ðV0 V1 Þ=V0 ; where V0 is original volume and V1 is volume after shrinkage. Area shrinkage: DA=A0 ¼ ðA0 A1 Þ=A0 ; where A0 is original volume and A1 is volume after shrinkage. Linear shrinkage: DL=L0 ¼ ðL0 L1 Þ=L0 ; where L0 is original volume and L1 is volume after shrinkage. 1. Volumetric shrinkage as function of linear shrinkage: V0 DV ¼ ðL0 DLÞ3 and V0 ¼ L30 ¼ >
DV=V0 ¼ 1 ð1 DL=L0 Þ3 ¼ 1 ðL0 =L1 Þ3 ¼ 3DL=L0 3ðDL=L0 Þ2 þ ðDL=L0 Þ3 DV=V0 w3DL=L0 if linear shrinkage L=L0 is small 2. Volumetric shrinkage as function of area shrinkage: V0 DV ¼ ðA0 DAÞ3=2 and V 0 ¼ A0
DV=V0 ¼ 1 ð1 DA=A0 Þ ¼ 1 ðA0 =A1 Þ3=2 DV=V0 w3=2DA=A0 if area shrinkage A=A0 is small 3=2
3. Area shrinkage as function of linear shrinkage: A0 DA ¼ ðL0 DLÞ2 and A0 ¼ L20 ¼ >
DA=A0 ¼ 1 ð1 DL=L0 Þ2 ¼ 1 ðL0 =L1 Þ2 ¼ 2DL=L0 ðDL=L0 Þ2 DA=A0 w2DL=L0 if linear shrinkage L=L0 is small
The Journal of Prosthetic Dentistry
Gibbs et al
% Volumetric shrinkage
8.0 7.0 *
6.0 5.0 4.0 3.0 2.0 1.0 0.0
GC Pattern Primopattern Primopattern Resin Gel Paste
3 Percentage volumetric shrinkage (mean and standard deviation) of tested pattern resins. Asterisk (*) indicates signiﬁcantly higher shrinkage. ANOVA followed by StudentNewman-Keuls post hoc test (a¼.05). Primopattern LC Paste, by contrast, uses different acrylates that may be responsible for the higher shrinkage value. The shrinkage values found for the Primopattern LC gel may also have been affected by the way the specimens were built and photopolymerized in one piece. To create thick layers, the manufacturer’s instruction manual recommends that each 1-mm layer of Primopattern LC gel be prepolymerized with a handheld light for 10 seconds or with a light-polymerizing unit for 1 minute. In this study, the specimens were light polymerized for 5 minutes in a Metalight Mini polymerization unit to obtain thorough photopolymerization. The measured shrinkage value of DuraLay was similar to the values from the only published study found11 that reported 6.5% volumetric shrinkage at 17 minutes and 7.9% after 24 hours of the DuraLay ‘standard’ mix (1.0 g powder to 0.8 mL liquid).11 In the present experiment, a ratio of 0.5 g powder to 0.3 mL liquid was used for DuraLay, which resulted in a volumetric shrinkage of 5.72% at 20 minutes. With less monomer, less shrinkage was found in the present study, as should be expected.
The manufacturer of GC Pattern Resin reported 0.36% shrinkage after 30 minutes and 0.37% shrinkage after 24 hours. These values are much lower than the values found in the present study. The manufacturer’s information did not contain details about the method used or even what shrinkage it was (volumetric or linear, postgel, or total). For example, if it was linear shrinkage, the value would be about 3 times less than the volumetric shrinkage. Also, postgel shrinkage values are likely to be considerably lower than total shrinkage values.16 Therefore, no meaningful comparison could be made between the data reported by the manufacturer and the data found in the present study. In this study, the volumetric shrinkage of GC Pattern Resin was 5.07%, similar to DuraLay (5.72%). The similarity in shrinkage found is supported by a previously published study that reported the same dimensional accuracy for these 2 resins.8 To date, no report of shrinkage values for Primopattern is available. The closest product with published shrinkage values was Primotec’s Primosplint, a photopolymerizing resin for an occlusal splint.12 The volumetric
ANOVA results for effect of pattern resin on volumetric shrinkage
Sum of Squares
Gibbs et al
shrinkage of Primosplint measured with a hydrostatic method was 5.1% with an irradiation time of 10 minutes and 5.2% with an irradiation time of 15 minutes.12 These values are close to the 5.42% of Primopattern Gel found in the present study. Other autopolymerizing and photopolymerizing resins for occlusal splints had volumetric shrinkage ranging from 4.5% to 6.4%.12 This study introduced a straightforward methodology to measure polymerization shrinkage. The results with this methodology are similar to reported volumetric shrinkage values.11,12 Conventional dilatometer and hydrostatic shrinkage measurement techniques supposedly provide a ‘free’ shrinkage value, which means that the specimens shrink without any hindering effect from the surrounding media. In the present study, a silicone platform was chosen to prevent the specimens from sticking to the platform during shrinkage, thus allowing it to contract freely. Other platform materials are also feasible, as long as the pattern resin does not stick and the surface is very smooth. The silicone impression material fulﬁlled the nonstick requirement and could be made very smooth by letting it set against a glass plate. Another challenge for capturing the prepolymerization image of autopolymerizing materials is that the transfer from the mixing to the measuring stage will take some time, during which the material may already start shrinking. All shrinkage methods have this limitation. For example, Mojon et al11 started capturing the data 2 minutes after the beginning of mixing. The simplicity of the method used in this study may reduce the time between mixing and the ﬁrst ‘prepolymerization’ shrinkage measurement. In this study, the prepolymerization image was captured 1 minute and 30 seconds after the start of mixing. For the photopolymerizing resins, there may also be an effect of premature polymerization due to ambient light. This limitation is also true for other testing methods if they are carried out in laboratories not equipped with blue-light (320 to 500 nm) blocking ﬁlters. However, the manufacturer of Primopattern claims that the photopolymerizing
Volume materials have a working time of greater than 20 minutes; thus the effect of premature polymerization from ambient light can likely be considered minimal. In the current study the shrinkage was determined immediately after setting, which was 20 minutes for the autopolymerizing and 5 minutes for the photopolymerizing materials. These times were chosen because pattern resins are usually used immediately after setting. However, the method that was developed for this study does allow follow-up measurements in future studies to determine the dimensional stability of pattern resin devices used directly after fabrication versus using the device several days/weeks after fabrication, provided laboratory temperature effects are controlled. Understanding the dimensional stability of pattern resins will help with material selection and handling to improve the ﬁt of implant prostheses.
CONCLUSIONS Within the limitations of this in vitro study, a photopolymerizing Primopattern LC Gel had volumetric shrinkage similar to those of the autopolymerizing pattern resins DuraLay and GC Pattern Resin. However, another photopolymerizing pattern resin, Primopattern LC Paste, has signiﬁcantly higher polymerization shrinkage than all other materials tested. The higher shrinkage may affect the accuracy of implant prosthesis fabrication.
REFERENCES 1. Wee AG, Aquilino SA, Schneider RL. Strategies to achieve ﬁt in implant prosthodontics: a review of the literature. Int J Prosthodont 1999;12:167-78.
2. Kan JY, Rungcharassaeng K, Bohsali K, Goodacre CJ, Lang BR. Clinical methods for evaluating implant framework ﬁt. J Prosthet Dent 1999;81:7-13. 3. Romero GG, Engelmeier R, Powers JM, Canterbury AA. Accuracy of three corrective techniques for implant bar fabrication. J Prosthet Dent 2000;84:602-7. 4. Vigolo P, Majzoub Z, Cordioli G. Evaluation of the accuracy of three techniques used for multiple implant abutment impressions. J Prosthet Dent 2003;89:186-92. 5. Naconecy MM, Teixeira ER, Shinkai RS, Frasca LC, Cervieri A. Evaluation of the accuracy of 3 transfer techniques for implantsupported prostheses with multiple abutments. Int J Oral Maxillofac Implants 2004;19:192-8. 6. Vigolo P, Fonzi F, Majzoub Z, Cordioli G. An evaluation of impression techniques for multiple internal connection implant prostheses. J Prosthet Dent 2004;92:470-6. 7. Primotec. Primopattern light cured universal modeling resin. Available at: http://www. primotecusa.com/product/primopattern. Accessed August 16, 2013. 8. Cho GC, Chee WW. Efﬁcient soldering index materials for ﬁxed partial dentures and implant substructures. J Prosthet Dent 1995;73:424-7. 9. Dumbrigue HB, Gurun DC, Javid NS. Prefabricated acrylic resin bars for splinting implant transfer copings. J Prosthet Dent 2000;84:108-10. 10. McDonnell T, Houston F, Byrne D, Gorman C, Claffey N. The effect of time lapse on the accuracy of two acrylic resins used to assemble an implant framework for soldering. J Prosthet Dent 2004;91: 538-40. 11. Mojon P, Oberholzer JP, Meyer JM, Belser UC. Polymerization shrinkage of index and pattern acrylic resins. J Prosthet Dent 1990;64:684-8. 12. Danesh G, Lippold C, Mischke KL, Varzideh B, Reinhardt KJ, Dammaschke T, Schäfer E. Polymerization characteristics of light- and auto-polymerizing resins for individual splints. Dent Mater 2006;22: 426-33. 13. Cerqueira NM, Ozcan M, Gonçalves M, da Rocha DM, Vasconcellos DK, Bottino MA, et al. A strain gauge analysis of microstrain induced by various splinting methods and acrylic resin types for implant impressions. Int J Oral Maxillofac Implants 2012;27: 341-5.
The Journal of Prosthetic Dentistry
14. GC. GC Pattern Resin LS low shrinkage modelling resin tips and tricks: technique and handling of GC Pattern Resin. 2009. p. 1-12. Available at: http://www.gcamerica.com/lab/products/ PATTERN_RESIN_LS/pattern_resin_tech_ guide.pdf. Accessed August 26, 2013. 15. Versluis A, Tantbirojn D. Relationship between shrinkage and stress. In: Daskalaki A, editor. Dental computing and applications: advanced techniques for clinical dentistry. Hershey: IGI Global; 2009. p. 45-64. 16. Tantbirojn D, Pfeifer CS, Braga RR, Versluis A. Do low-shrink composites reduce polymerization shrinkage effects? J Dent Res 2011;90:596-601. 17. Penn RW. A recording dilatometer for measuring polymerization shrinkage. Dent Mater 1986;2:78-9. 18. Puckett AD, Smith R. Method to measure the polymerization shrinkage of light-cured composites. J Prosthet Dent 1992;68:56-8. 19. de Gee AF, Feilzer AJ, Davidson CL. The linear polymerization shrinkage of unﬁlled resins and composites determined with a linometer. Dent Mater 1993;9:11-4. 20. Sharp LJ, Choi IB, Lee TE, Sy A, Suh BI. Volumetric shrinkage of composites using video-imaging. J Dent 2003;31:97-103. 21. Reliance Dental Mfg Co. DuraLay inlay pattern resin: brush method. p. 1-3. Available at: http://reliancedental.net/yahoo_site_ admin/assets/docs/duralay.71185857.pdf. Accessed August 26, 2013. 22. Mosch J, Hoffmann A. One for all - efﬁcient modeling made easy. Spectrum Dialogue 2010;9:76-82. Available at: http:// primotecusa.com/sites/default/ﬁles/ downloads/PUB1001-US-One-for-AllEfﬁcient-Modeling-Made-Easy.pdf. Accessed August 16, 2013.
Corresponding author: Dr Swati Ahuja University of Tennessee Health Science Center 875 Union Ave, Memphis, TN 38163 E-mail: [email protected]
Acknowledgments The authors thank Drs David Cagna, Greg Paprocki, and Vinay Jain for their contributions in the development of this study. The authors thank Primotec, Westport, Conn, for providing material support. Copyright ª 2014 by the Editorial Council for The Journal of Prosthetic Dentistry.
Gibbs et al